From One-Dimensional Linear Chain to Two-Dimensional Layered Chalcogenides XBi4S7(X = Mn, Fe): Syntheses, Crystal and Electronic Structures, and Physical Properties
Luo, Zhong-Zhen; Lin, Chen-Sheng; Cheng, Wen-Dan; Zhang, Wei-Long; Li, Yuan-Bing; Yang, Yi; Zhang, Hao; He, Zhang-Zhen; Crystal Growth & Design 13 (2013) 4118–; doi:10.1021/cg4009398

data_4508260
_publ_section_title
;
 From One-Dimensional Linear Chain to Two-Dimensional Layered
 Chalcogenides XBi4S7(X = Mn, Fe): Syntheses, Crystal and Electronic
 Structures, and Physical Properties
;
_journal_issue                   9
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              4118
_journal_paper_doi               10.1021/cg4009398
_journal_volume                  13
_journal_year                    2013
_chemical_formula_sum            'Bi4 Mn S7'
_chemical_formula_weight         1115.35
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 104.755(14)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   12.916(12)
_cell_length_b                   3.970(3)
_cell_length_c                   11.831(10)
_cell_measurement_reflns_used    835
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4816
_cell_measurement_theta_min      3.2622
_cell_volume                     586.6(9)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  Saturn724+
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0794
_diffrn_reflns_av_sigmaI/netI    0.1218
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -4
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            2586
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         3.26
_diffrn_standards_number         773
_exptl_absorpt_coefficient_mu    62.023
_exptl_absorpt_correction_T_max  0.000
_exptl_absorpt_correction_T_min  0.000
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.314
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Prism
_exptl_crystal_F_000             938
_exptl_crystal_size_max          0.1800
_exptl_crystal_size_mid          0.1700
_exptl_crystal_size_min          0.1300
_refine_diff_density_max         2.964
_refine_diff_density_min         -3.561
_refine_diff_density_rms         0.758
_refine_ls_extinction_coef       0.00065(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.805
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     40
_refine_ls_number_reflns         770
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.805
_refine_ls_R_factor_all          0.0686
_refine_ls_R_factor_gt           0.0370
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0000P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0674
_refine_ls_wR_factor_ref         0.0826
_reflns_number_gt                534
_reflns_number_total             775
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg4009398_si_002.cif
_cod_data_source_block           compd1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        586.7(9)
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               4508260